# Polymer Chemistry. The Basic Concepts - Himenz P.C.

**Download**(direct link)

**:**

**162**> 163 164 165 166 167 168 .. 312 >> Next

we write

2fkd[l] = 2kt[M*]s2

(6.22)

Termination

363

or

/ f ê V/2

lM',s = \ir) [I1*

(623)

This important equation shows that the stationary-state free-radical

concentration increases with [I]1/2 and varies directly

with kd1/2 and inversely with ê{1/2.

The concentration of free radicals determines the rate at which polymer

forms and the eventual molecular weight of the polymer, since each

radical is a growth site. We shall examine these aspects of Eq. (6.23) in

the next section. We conclude this section with a numerical example which

concerns the stationary-state radical concentration for a typical system.

Example 6.2

For an initiator concentration which is constant at [I]0, the non-

stationary-state radical concentration varies with time according to the

following expression:

[M-] = exp[(16fkdkt[I]0)1/2t] - 1

[M ] s exp[(16fkdkc [I]0)1/2t] + 1

Calculate [M-]s and the time required for the free-radical concentration

to reach 99% of this value using the following as typical values for

constants and concentrations: kd = 1.0 X 10~4 sec"1, kt = 3 X 107 liter

mol"1 sec"1, f = lA, and [I] î = 10~3 M. Comment on the assumption [I] =

[I]0 that is made in deriving the non-stationary-state equation.

Solution

Use Eq. (6.23) to evaluate [M-]s for the system under consideration:

/fkd \1/2 /ÑË)(1.0Õ 10~4)(10"3) \1/2

[ì']' = Kl,4 -( .................Ø"' ) ¦ 0-"x .o-V

= 4.08 X 10"8 mol liter"1

This low level of concentration is typical of free-radical

polymerizations. Next we inquire how long it will take the free-radical

concentration to reach

0.99[M-]S, or 4.04 X 10~8 mol liter-1 in this case. Let a = (16fkdkt [I]

0)1/2 and rearrange the expression given to solve for t when [M ] / [M •]

s = 0.99:

0.99(eat + 1) = eat - 1, or 1 + 0.99 = eat(l - 0.99). Therefore the

product at = ln(l .99/0.01) = In 199 = 5.29, and a = [16(^)(1.0 X 10"4)(3

X 107) (10"3)]1/2 = 4.90 sec"1. Hence t = 5.29/4.90 = 1.08 sec. This

short period is also typical of the time required to reach the stationary

state.

364

Addition or Chain-Growth Polymerization

The assumption that [I] = [I]0 may be assessed by examining the

integrated form of Eq. (6.2) for this system and calculating the ratio

[I]/[I]0 after 1.08 sec:

In | JjyLj = -kdt = -(1.0 X 10~4)(1.08) = -1.08 X 10~4

-Ô- = 0.99989

[I] î

Over the time required to reach the stationary state, the initiator

concentration is essentially unchanged. As a matter of fact, it would

take about 100 sec for [I] to reach 0.99[I]0 and about 8.5 min to reach

0.95[I]0, so the assumption that [I] = Øî is entirely justified over the

short time involved.

6.5 Propagation

The propagation of polymer chains is easy to consider under stationary-

state conditions. As the preceding example illustrates, the stationary

state is reached very rapidly, so we lose only a brief period at the

start of the reaction by restricting ourselves to the stationary state.

Of course, the stationary-state approximation breaks down at the end of

the reaction also, when the radical concentration drops toward zero. We

shall restrict our attention to relatively low conversion to polymer,

however, to avoid the complications of the Tromms-dorff effect. Therefore

deviations from the stationary state at long times need not concern us.

Consideration of reaction (6.B) leads to

= kptMHM]

(6.24)

as the expression for the rate at which monomer is converted to polymer.

In writing this expression, we assume the following:

1. The radical concentration has the stationary-stage value given by

Eq. (6.23).

2. kp is a constant independent of the size of the growing chain and

the extent

of conversion to polymer.

3. The rate at which monomer is consumed is equal to the rate of polymer

formation Rp:

-d[M] = d[polymer] _ R

^ 25)

Propagation

365

Combining Eqs. (6.23) and (6.24) yields

_ _ 1A . .,

Rp = kp[M] ,/* = êàðð[Ì][1]é

(6.26)

in which the second form reminds us that an experimental study of the

rate of polymerization yields a single constant (subscript app) which the

mechanism reveals to be a composite of three different rate constants.

Equation (6.26) shows that the rate of polymerization is first order in

monomer and half order in initiator and depends on the rate constants for

each of the three types of steps-initiation, propagation, and

termination-that make up the chain mechanism. Since the concentrations

change with time, it is important to realize that Eq. (6.26) gives an

instantaneous rate of polymerization at the concentrations considered.

**162**> 163 164 165 166 167 168 .. 312 >> Next